- Home
- Documents
*Influence of the Butt Joint Design of TIG Welding on the Thermal Stresses- Hani Aziz Ameen*

prev

next

out of 18

View

350Category

## Documents

Embed Size (px)

DESCRIPTION

welding, butt joint, TIG, MIG, TIG/MIG, thermal stresses, Hani Aziz Ameen, ANSYS, finite element method

Eng. & Tech. Journal, Vol.29, No.14, 2011

Influence of the Butt Joint Design of TIG Welding on the Thermal StressesDr. Hani Aziz Ameen*, Khairia Salman Hassan** & Muwafaq Mehdi Salah**Received on: 24/2/2011 Accepted on: 8/9/2011

Abstract The aim of this paper is to demonstrate the influence of the single butt joint design of TIG welding on the thermal stresses for carbon steel type St-37. The butt welding was performed by V angles 30,45,60 and 90 and the thermal stresses analysis is based on the local moving heat flux. The numerical model developed by ANSYS12 software based on solving the three dimensional energy equation, considering moving heat source and temperature dependent material properties. Temperature and stresses distributions were obtained function of time. From the results, it is evident that the joint design has an important role in the welding process, when the edge angle of the welding region gets bigger, the faults get less due to increase of heat flux in the welding region. It can be concluded that the specimen with less than 6mm thickness can be welded without edge angle preparation, due to increase the thermal stresses when edge angle is evident and higher thermal stresses distribution was at edge angle 60 and lowest thermal stresses distribution was at 90. Keywords: Welding technology, Finite element method, Moving heat source, ANSYS12 software.

St-37 (30,45,60,90)V . ANSYS12 . . . 6 .90 06

* Technical College, Foundation of Technical Education /Baghdad ** Institute of Technology, Foundation of Technical Education /Baghdad 2841

PDF created with pdfFactory Pro trial version www.pdffactory.com

Eng. & Tech. Journal, Vol.29, No.14, 2011

Influence of the Butt Joint Design of TIG Welding on the Thermal Stresses

Introduction IG butt welding is a process that is being widely used in industry for sheet joining purposes. Many applications of welding made of carbon steel (e.g. bridge structure, fuel tanks ..etc) are subjected to various stresses (mechanical, thermal ..etc). The toughness and resistance of the welded piece to failure depending on many factors such as shape, design of the welding piece, the method implemented for welding and the nature of the applied stresses. Estimation of the temperature field within a metal plate produced by a moving heat source subjected on its surface is obviously of a great practical interest for the study of welding processes. It is well known that the welding process relies on an intensely localized heat input, which tends to generate undesired residual stresses and deformations in welded structures, especially in the case of thin plates[1]. Therefore, estimating the magnitude of welding deformations and characterizing the effects of the welding conditions are deemed necessary. With modern computing facilities, the finite element technique has become an effective method for prediction and assessment of welding stresses[2]. Therefore, rapidly and accurately predicting welding induced distortion for real engineering applications is more challenging. Hani [3] (1998) explains the thermomechanical model which was developed using FE method to calculate temperature, stresses and distortions during elasto-plastic analysis. Lindergen et al [4] (2002) presented a thermo-mechanical Analysis in butt welding of copper canister for spent nuclear fuel. Anas

T

And Abid [5] (2004) studied the finite element volume for modeling welds and it depicts a brief history of the Simulation of welds. Dragi and Ivana [6] (2009) studied the finite element analysis of residual stresses in butt welding of two similar plates. Hani and Khaiyria [7] (2010) studied experimentally and numerically the influence of single butt MIG welding shapes design on the microstructure and stresses of low carbon steel. Karima et al (2010) [8] studied the thermal distribution within metal plate subjected to moving heat source using finite element method. Many analytical 2D or 3D models have been developed in literatures [9,10,11,12] using integral transformations (a finite cosine Fourier integral transform), separation of variables and Jaeger's classical heat source method respectively. These models are principally based on several postulates regarding source term modeling methods (shape, source, distribution of energy) with or without surface cooling. The objective of this work is to study the thermal stresses of two metal plate subjected to a moving heat source during TIG welding process with different shape design. Experimental Choice of Metals Low carbon steel St37 was chosen according to the Russian Standards (Gost) . Its chemical analysis is shown in Table (1). Preparation of welding piece - Selection metallic plates, 5 mm thick, 100 mm long and 30 mm wide. - making preparation single V angle of 30. - The operation is repeated on the remaining pieces to make V angles of (45, 60 and 90).2842

PDF created with pdfFactory Pro trial version www.pdffactory.com

Eng. & Tech. Journal, Vol.29, No.14, 2011

Influence of the Butt Joint Design of TIG Welding on the Thermal Stresses

Welding Process Welding is done by electric arc (TIG) on the piece. The conditions for the process are indicated in Table(2) .The Input heat quantity is calculated by the following equation[1]: IV 60 (1) Heat Input = S where I .. current (amp.) , V.. Voltage (volt) , and S.. welding speed (m/min) Welding Electrode The welding electrode (316L) is used [13,14] with 2.8 mm diameter in which the chemical composition is shown in Table(3). Classification of specimens After preparation, the specimens were classified in the groups as shown below. A B C D Butt welding single angle 30 Butt welding single angle 45 Butt welding single angle 60 Butt welding angle 90

thermal conductivity of the metal. During phase transformation (i.e melting or solidification) then

q = H

fs t

where H is the latent

heat of fusion and .. density. Discretizition of equation(2) is adopted with FEM to give elemental matrices and vector. The assembly of these elemental matrices into global matrices and vector give first order transient simultaneous differential equations [3,15]: Finally the plate surface exposed to specified heat flux qs , can be formulated mathematically across the central segment of the upper surface as:

(4) The elemental matrices and vector can be computed from: C e = cN i N j d (5) ije

T1 plate = q s y & CT + KT = F =

(3)

Mathematical Model Conservation of Energy The three dimensional energy equation for an isotropic material is used to describe the plate thermal history [8,15].

N Nj Ni Nj (6) Ke = i ij x x + y y d+ S hNi Njd e e

Fie = N i h T dSe

(7)

2T 2T 2T q 1 T + + + = x2 y 2 z 2 t(2) where is the thermal diffusivity of the metal at time t internal heat source per unit volume (existed when the is phase transformation otherwise it is vanished.

q

Finite Element Model The general purpose FE package ANSYS12 is used for both the thermal and stress analyses performed directly with an appropriate couple elements [7,16]. The main features of the 3D model are the moving heat input, the element birth-and-death technique, the heat loss, the temperature-dependent material properties, and the application of ANSYS parametric design language (APDL) to model the moving heat source and adaptive boundary conditions (Appendix-A-). The element types used in the thermal and structural2843

PDF created with pdfFactory Pro trial version www.pdffactory.com

Eng. & Tech. Journal, Vol.29, No.14, 2011

Influence of the Butt Joint Design of TIG Welding on the Thermal Stresses

analyses are SOLID5 (Fig-1-). It is the 8-noded brick elements. The direct generation meshes used is shown in Fig.2 for different shapes design. The moving heat source is modeled by setting a heat flux to the elements of the fusion zone. The total heat input is evaluated according to the equation(1). The metal deposition is considered by using the element birth technique. This technique is based on deactivating and reactivating the elements of the fusion metal at a prescribed time as the deposition progresses. This is also the arrival time for the heat input for the deposited elements. Consequently, the thermal mass and the heat flow conditions accurately portray the sequential deposition of the material. As it was mentioned earlier, the boundary conditions include convective heat loss. Since only the current outer surface of the partially completed deposit is a convecting surface at any given time, the boundary conditions are subject to the birth-death option. Also, the boundary conditions depend strongly on the position of the heat source[17]. The ANSYS steps can be demonstrated by our developed APDL program (Appendix -A-) to make the butt welding analysis. Results and Discussion By observed and calculated heat quantity as shown in Table (2), it is found that with increasing preparation edge angle of the welded plates, the heat quantity decrease, quantity of welding metal decreases, welding region possesses better quantities, greater heat transfer to adjoining region (which is effected directly by heat), while it can be shown that the heat quantity is equal with weld edge 30 V and 90 V, this is due to the same input parameters. Increasing of heat quantity contributes in growth of granules volume with high ductility due to slow2844

cooling of the metal during welding as well as weak mechanical properties (resistance to tension and hardness). Therefore, it is preferred that the welding angle be 30o and 90 for homogenous heat

Recommended

View more >